9}$Fe$_{0.1}$O$_3$.

CONCLUSIONS
===========

The electronic structures of of multiferroic oxides of Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ ($0 \le x \le 0.12$). have been investigated by employing synchrotron-radiation excited PES and XAS. Via Fe and Ti $2p$ XAS measurements, the valence states of Fe and Ti ions have been determined experimentally. The valence states of Fe ions are found to be Fe$^{2+}$-Fe$^{3+}$ mixed-valent for $x>0$ but nearly trivalent for $x$=0. The valence states of Fe ions are found to decreases from being nearly trivalent for $x$=0 ($v$(Fe)$\sim 3$) to $v$(Fe)$\sim 2.6$ for $x$=0.12. The valence states of Ti ions do not change with $x$ for $x \le 0.12$, and stay being tetravalent (Ti$^{4+}$). The valence states of Ba ions are close to being divalent (Ba$^{2+}$) and remain unchanged for $x \le 0.12$. The decreasing trend of valence states of Fe ions in Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ with $x$ will play an important role in the electronic and magnetic properties of this system.

This work was supported by the NRF under Contract No. 2014R1A1A2056546, and in part by the Research Fund, 2015 of the Catholic University of Korea. Experiments at PLS were supported by MSIP and PAL.

Y. Tokura and S. Seki, Advanced Materials [**22**]{}, 1554 (2010). Y. Kimura, T. Goto, H. Shintani, K Ishizaka, T. Arima and Y. Tokura, Nature [**426**]{}, 55 (2003). N. Ikeda, H. Ohsumi, K. Ohwada, K. Ishii, T. Inami, K. Kakurai, Y. Murakami, K. Yoshii, S. Mori, Y. Horibe and H. Kito, Nature (London) [**436**]{}, 1136 (2005). A. Rajamani, G. F. Dion
9}$Fe$_{0.1}$O$_3$. 

 CONCLUSIONS 
 = = = = = = = = = = = 

 The electronic structures of of multiferroic oxides of Ba$_{1 - x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3 $ ($ 0 \le x \le 0.12 $). have been investigated by use synchrotron - radiation sickness excited PES and XAS. Via Fe and Ti $ 2p$ XAS measurements, the valence states of Fe and Ti ion have been determined experimentally. The valence states of Fe ions are establish to be Fe$^{2+}$-Fe$^{3+}$ mixed - valent for $ x>0 $ but nearly trivalent for $ x$=0. The valence states of Fe ions are found to decrease from being nearly trivalent for $ x$=0 ($ v$(Fe)$\sim 3 $) to $ v$(Fe)$\sim 2.6 $ for $ x$=0.12. The valence states of Ti ion do not change with $ x$ for $ x \le 0.12 $, and stay being tetravalent (Ti$^{4+}$). The valence states of Ba ions are close to being divalent (Ba$^{2+}$) and remain unaltered for $ x \le 0.12$. The decreasing trend of valence states of Fe ion in Ba$_{1 - x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3 $ with $ x$ will play an important role in the electronic and magnetic properties of this arrangement. 

 This work was supported by the NRF under Contract No. 2014R1A1A2056546, and in part by the Research Fund, 2015 of the Catholic University of Korea. Experiments at PLS were support by MSIP and PAL. 

 Y. Tokura and S. Seki, Advanced Materials [ * * 22 * * ] { }, 1554 (2010). Y. Kimura, T. Goto, H. Shintani, K Ishizaka, T. Arima and Y. Tokura, Nature [ * * 426 * * ] { }, 55 (2003). N. Ikeda, H. Ohsumi, K. Ohwada, K. Ishii, T. Inami, K. Kakurai, Y. Murakami, K. Yoshii, S. Mori, Y. Horibe and H. Kito, Nature (London) [ * * 436 * * ] { }, 1136 (2005). A. Rajamani, G. F. Dion
9}$Fe$_{0.1}$O$_3$.

FONCLUSIONS
===========

The electronig structures of of multmferroid oxides of Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ ($0 \le x \le 0.12$). hate bwen ibvestigated by employivg synchrltron-raduatiib excited 'SS and WCS. Viz Fe cnv Ti $2p$ XAS measorements, the valence statev uf Fe and Ti ions have been determineq experomfntally. The vajenct seatea of Fe ions are found to be Fe$^{2+}$-Fe$^{3+}$ jixed-vanent for $x>0$ buy nearly trivalent for $x$=0. Tje vwlence states of Ff ions are dounq to decreaser from being nearly trjvalent for $x$=0 ($v$(Fe)$\sim 3$) to $v$(Fe)$\sim 2.6$ for $x$=0.12. The valguxe djates of Ti mons dj not change with $x$ xor $x \lr 0.12$, and stay belng txtracalent (Ti$^{4+}$). The valence states of Ba ions are closa co being divalent (Ba$^{2+}$) qne remdin gnchxbgea fkr $x \le 0.12$. Tje vecreasing frend of vaoence states of Fe oogw in Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Re$_{0.1}$O$_3$ wieh $x$ will play an important role in the enecfronic and magnetic properties of this systel.

This worh was supported by the NRF under Contract No. 2014R1A1A2056546, dnd ii oaru nn thd Rfsearch Fund, 2015 of the Catholic University of Kjdes. Vxperiments at PLF were suppprhec by MSIP and KAL.

Y. Tokurz and S. Seki, Advanfed Matgrials [**22**]{}, 1554 (2010). Y. Kimtra, Y. Goto, H. Shintani, K Ishizakq, T. Arima anb Y. Tokura, Nature [**426**]{}, 55 (2003). U. Ikeda, H. Ohrumi, K. Oheada, K. Ishii, T. Inami, K. Yakudai, Y. Murakwmi, K. Yosgki, S. Mori, Y. Horice sng H. Kito, Nature (London) [**436**]{}, 1136 (2005). W. Rajamanm, G. F. Dion
9}$Fe$_{0.1}$O$_3$. CONCLUSIONS =========== The electronic structures of oxides Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ ($0 x \le 0.12$). synchrotron-radiation PES and XAS. Fe and Ti XAS measurements, the valence states of and Ti ions have been determined experimentally. The valence states of Fe ions found to be Fe$^{2+}$-Fe$^{3+}$ mixed-valent for $x>0$ but nearly trivalent for $x$=0. The states Fe are to decreases from being nearly trivalent for $x$=0 ($v$(Fe)$\sim 3$) to $v$(Fe)$\sim 2.6$ for $x$=0.12. The states of Ti ions do not change with for $x \le 0.12$, stay being tetravalent (Ti$^{4+}$). The states Ba ions close being (Ba$^{2+}$) and remain for $x \le 0.12$. The decreasing trend of valence states of Fe ions in Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ with $x$ play an in the and properties this system. This supported by the NRF under Contract in part by the Research Fund, 2015 of Catholic University Korea. Experiments at PLS were supported MSIP and PAL. Y. Tokura and S. Seki, Materials [**22**]{}, 1554 (2010). Y. Kimura, T. Goto, H. Shintani, K Ishizaka, T. Arima and Nature [**426**]{}, 55 (2003). Ikeda, H. Ohsumi, Ohwada, Ishii, Inami, Kakurai, Y. K. Yoshii, S. Mori, Y. Horibe and H. Kito, Nature (London) 1136 (2005). A. Rajamani, G. F. Dion
9}$Fe$_{0.1}$O$_3$.

CONCLUSIONS
===========

The electronIc structurEs of oF muLtiFeRroiC oxiDes of Ba$_{1-x}$Bi$_x$Ti$_{0.9}$FE$_{0.1}$o$_3$ ($0 \le x \Le 0.12$). have been investigated By empLoYIng sYNcHrotrOn-radiaTIoN EXciTeD PeS aNd xaS. via Fe And ti $2p$ XAS mEasurementS, thE vAlence states OF FE and Ti ions HavE been determiNed ExperiMeNtaLLy. The ValEnce sTates oF fe ions Are found tO bE fe$^{2+}$-Fe$^{3+}$ miXEd-valenT FOr $X>0$ but Nearly trivalent foR $X$=0. THE valence states Of Fe ioNs ARe FOUnd To dEcreases frOm Being NEarly trIVaLENT foR $X$=0 ($v$(Fe)$\sim 3$) to $v$(Fe)$\sIm 2.6$ for $x$=0.12. The vaLEncE stateS oF Ti IOns do nOt chaNgE WitH $x$ for $x \le 0.12$, and Stay Being tetrAvalenT (ti$^{4+}$). The vaLEnce staTes of BA ioNs aRe clOSe To BeiNg DIvaLEnT (Ba$^{2+}$) ANd rEmain uncHaNgEd for $X \le 0.12$. THE DECreaSinG treNd of vAlence states oF Fe Ions IN Ba$_{1-X}$Bi$_x$TI$_{0.9}$Fe$_{0.1}$O$_3$ wIth $x$ WiLl plaY an impOrtanT rOle in the electroNic aNd magnetiC prOpErtIeS of thIS systeM.

ThIs wOrk was sUpporteD By tHe nrf UnDer Contract No. 2014R1A1A2056546, anD iN PArT by the ReSearch fUnD, 2015 oF The CathoLiC UnIverSITy of KOrea. eXpEriments At PLS wERe SuPported By mSIP anD PaL.

Y. tokUra anD s. SekI, AdvanCed MaterIals [**22**]{}, 1554 (2010). Y. kImura, T. Goto, H. ShiNTani, K Ishizaka, t. arIMA aND Y. ToKurA, Nature [**426**]{}, 55 (2003). N. IkeDa, H. OHSumi, k. OhwADa, k. IsHIi, T. InAmi, K. KAkURaI, y. Murakami, K. Yoshii, S. MoRi, y. HoribE and H. kito, Nature (LonDon) [**436**]{}, 1136 (2005). A. RajamaNI, g. f. Dion
9}$Fe$_{0.1}$O$_3$.

CONCL USIONS
=== ===== === 

T he  ele ctro nic structures of o f multiferroic oxidesof Ba $_ { 1-x} $ Bi $_x$T i$_{0.9 } $F e $ _{0 .1 }$ O$_ 3$ ($ 0 \le  x\le 0.1 2$). havebee ninvestigated by  employing  sy nchrotron-ra dia tion e xc ite d  PESand  XAS.  Via F e  and T i $2p$ XA Sm easure m ents, t h e  v alen ce states of Fe a n dT i ions have be en det er m in e d  ex per imentally.  T he va l ence st a te s o f F e  ions are fou nd to be Fe $ ^{2 +}$-Fe $^ {3+ } $ mixe d-val en t  fo r $x>0$ but  nea rly triva lent f o r $x$=0 .  The va lencesta tes  ofF eio nsar e  fo u nd  to dec reases f ro mbeing  nea r l y triv ale nt f or $x $=0 ($v$(Fe)$ \si m 3$ )  to  $v$( Fe)$\ sim2. 6$ fo r $x$= 0.12.  T he valence stat es o f Ti ions  do  n otch angew ith $x $ f or$x \le0.12$,a ndst a y be ing tetravalent (T i$ ^ { 4+ }$). The  valen c est a tes of B aion s ar e close  tob ei ng dival ent (B a $^ {2 +}$) an dremain  u nch ang ed fo r  $x\le 0. 12$. The  decr e asing trend of valence state s  o f Fe ions  in  Ba$_{1-x}$ Bi$_ x $Ti$ _{0. 9 }$ Fe$ _ {0.1} $O$_3 $w it h  $x$ will play an i mp ortant  role  in the elect ronic andm a g netic pr oper t ie s  of this syste m.

T his work w a s suppor ted b y the NR F under C o n tract No . 2 014 R1A 1A2 0 5 65 46, and in pa r t  byth e Resea rch  Fund,201 5 o f t heCa tholic Un iversity  o fKo re a.Exper i ments at  P LSwe resuppo r ted by  MSIP  and  P AL . 

Y . Tokur a  a n d  S.Se ki , Ad van ce d Mat eria l s [ **22**] {}, 1554(20 1 0).Y.  K imura,T. Goto, H. S hi ntani, K I sh iza ka, T. A rima and  Y. Tokura, Nature [**4 2 6**]{},  55  (200 3).N. Ikeda,  H.  Ohsum i,K . Ohwa da, K.  Ishi i,  T. I nami, K .Kak ur ai, Y. Mur a k ami , K.Yo shii , S. Mo ri, Y. Horibe andH . K ito, Nature ( Lon don) [ ** 436 * *] { },11 3 6 ( 2 0 05). A. Rajaman i, G. F. D io n 
9}$Fe$_{0.1}$O$_3$.

CONCLUSIONS
===========

The electronic_structures of_of multiferroic oxides of_Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$ ($0_\le_x \le_0.12$)._have been investigated_by employing synchrotron-radiation_excited PES and XAS._Via Fe and_Ti_$2p$ XAS measurements, the valence states of Fe and Ti ions have been determined_experimentally._The valence_states_of_Fe ions are found to_be Fe$^{2+}$-Fe$^{3+}$ mixed-valent for $x>0$_but nearly_trivalent for $x$=0. The valence states of Fe_ions_are found to_decreases from being nearly trivalent for $x$=0 ($v$(Fe)$\sim 3$)_to $v$(Fe)$\sim 2.6$ for $x$=0.12. The_valence states of_Ti_ions_do not change with_$x$ for $x \le 0.12$, and_stay being tetravalent (Ti$^{4+}$). The valence_states of Ba ions are close to_being divalent (Ba$^{2+}$) and remain unchanged_for $x \le 0.12$. The_decreasing trend_of valence states of Fe_ions in Ba$_{1-x}$Bi$_x$Ti$_{0.9}$Fe$_{0.1}$O$_3$_with $x$_will play an_important role in the electronic and_magnetic properties of_this system.

This work was supported by_the_NRF under Contract_No._2014R1A1A2056546,_and in_part by the_Research_Fund, 2015_of_the Catholic University of Korea. Experiments_at_PLS were supported by MSIP and PAL.

Y._Tokura and S. Seki,_Advanced_Materials [**22**]{}, 1554 (2010)._Y. Kimura, T. Goto, H._Shintani, K Ishizaka, T. Arima and_Y. Tokura,_Nature [**426**]{},_55 (2003). N. Ikeda, H. Ohsumi, K. Ohwada, K. Ishii, T._Inami, K. Kakurai, Y. Murakami, K._Yoshii, S. Mori, Y._Horibe and_H._Kito, Nature (London)_[**436**]{},_1136 (2005)._A. Rajamani, G. F. Dion